THE COMPRESSIVE STRENGTH PROPERTIES OF .the compressive strength properties of mineral wool slabs:
Embed Size (px)
Transcript of THE COMPRESSIVE STRENGTH PROPERTIES OF .the compressive strength properties of mineral wool slabs:
ISSN 13923730 print / ISSN 18223605 online
JOURNAL OF CIVIL ENGINEERING AND MANAGEMENThttp:/www.jcem.vgtu.lt
2007, Vol XIII, No 2, 97106
THE COMPRESSIVE STRENGTH PROPERTIES OF MINERAL WOOL SLABS: INFLUENCE OF STRUCTURE ANISOTROPY AND METHODICAL FACTORS
Andrius Buska1, Romualdas Maiulaitis 2 Dept of Building Materials, Vilnius Gediminas Technical University, Saul tekio al. 11, LT-10223 Vilnius,
Lithuania. E-mail: firstname.lastname@example.org; 2 email@example.com
Received 5 July 2006; accepted 7 Dec 2006
Abstract. This paper presents the research on the structure and compressive stress or compressive strength of mineral wool products. The products of chaotic, directional and combinative fibres structure have been studied visually and micro-scopically. During mechanical tests it was determined that compressive stress (compressive strength) of the stone wool products is dependent on the direction of the load working to the product major face, test specimen dimensions, force in-creasing rate, fibres distribution (orientation) and methodical peculiarities.
Keywords: mineral wool, stone wool, fibres, structure, compressive stress at 10 % relative deformation, compressive strength, deformation.
The thermal insulation products made of mineral wool depending on the orientation of fibres could be di-vided into the chaotic (the case when fibres are distrib-uted randomly and in different directions irregularly) and the directional (the case when fibres are distributed in a certain order) [1, 2] in terms of the structure. The mineral wool products which have the directional fibres structure are called lamella . Moreover, some products of the combinative fibres structure are used for certain construc-tions .
The dominating orientation of the fibres in the prod-ucts of the directional structure is perpendicular to the surface of the insulated enclosure construction (wall, roof or floor base). The products of the directional fibres structure may be formed by packing, cubic and corrugat-ing technology . However, most often such products are produced by regulating the fibres direction on the belt conveyor or by forming mineral wool semiproduct layer of certain dimensions by a conveyor method. After the layer is cut in strips of the width equal to the original product thickness, and finally the strips are rotated at 90 angle .
On the other hand, differences of the mechanical properties and deformation of the mineral wool products of the directional and random fibres structure appear to be not relevant. However, as construction practice shows, the contractors are often complaining about the irregular compressive stress (compressive strength) and deforma-tion of slabs used for facade and roof thermal insulation. The assumption may be made that the compressive strength and other mechanical properties of mineral wool products depend on fibre distribution (orientation) in the product structure, the direction of the load working to the product major face etc .
The dependence of thermal and other particular properties of the mineral wool on fibre orientation, length and shape is very well-known and successfully used in production technologies of thermal insulation, structural, refractory and compositional materials . A rela-tively large influence of the ambient temperature, test specimen strength and density, pressing of the measure-ment sensors to the test specimen on the coefficient of thermal conductivity of mineral wool products was de-termined during tests. Furthermore, according to the con-version formulas applied for this indicator, there are some application limits [16, 17]. However, there has been less research on influence of the same factors effecting the performance of thermal insulated materials (including stone wool), for instance, strength. In our opinion, this factor is insufficiently evaluated in the standards regulat-ing the mechanical properties of mineral wool products and their measurement  because some methodical aspects of standards (force increasing rate, dimensions of the test specimens and their preparation before testing) are not strictly defined, especially in standards of differ-ent countries.
In order to determine the influence of fibre orienta-tion in the product structure, the load direction in terms of the product in its intended use and some other methodical factors on the mechanical properties (compressive stress at 10 % relative deformation (10) and compressive strength (m)) of the mineral wool slabs produced by belt conveyor technology, the following aspects have to be analysed:
dependence of the product compressive stress on the test specimen dimensions and force increasing rate;
dependence of the product compressive stress on the load direction;
comparison of the product compressive stress with standards applicable in different countries.
A. Buska, R. Maiulaitis / JOURNAL OF CIVIL ENGINEERING AND MANAGEMENT 2007, Vol XIII, No 2, 97106
2. Test specimens and methods
2.1. Description of test specimens and testing equipment
Two types of the stone wool slabs produced by belt conveyor technology were used for testing:
1. 100130 kg/m3 density slabs with declared coeffi-cient of thermal conductivity D 0,039 W/(mK), whereas declared compressive stress at 10 % rela-tive deformation (10) 30 kPa. The dimensions of the factory-made slabs were 1000 600 100 mm. The amount of the organic content was determined by heating the slab fragments at 550 C for two hours. The measured amount 3,7 % (by mass). These test specimens were used by performing the re-
search on the dependence of compressive stress and de-formations of the mineral wool slabs according to the test specimen dimensions and force increasing rate (Chapter 3.3). The tests were performed by a universal electro-mechanic testing machine P-0,5 U4.2 (former USSR) and universal flexure/compression equipment ToniNorm (Toni technik Gmbh, Germany) with integrated data-processing program ToniTrol Expert (Fig 1).
Fig 1. A specimen under load in the test machine ToniNorm
2. 100150 kg/m3 density slabs with declared coeffi-cient of thermal conductivity D 0,039 W/(mK), whereas declared compressive stress at 10 % rela-tive deformation (10) 40 kPa. The dimensions of the factory-made slabs were 1000 500 100 mm. The amount of the organic content was determined by heating the slab fragments at 550 C for two hours. The measured amount was 4,5 % (by mass). These test specimens were used for the research on
the dependence of compressive stress values in the direc-tion of the load (Chapter 3.2) and comparable measure-ments of compressive stress by the standards of different countries (Chapter 3.4). Universal computer-integrated apparatus H 10 KS (Housfield, England) determining strength of the thermal insulated products were used (Fig 2).
Fig 2. Compression testing machine H 10 KS
The mineral wool fibre structure during the research
was studied visually and by optical and electronical mi-croscopes:
optical stereo binocular microscope SteddyT Bino 7300 with photo appendage (2,5...120);
electronical microscope JEOL JSM5600 (maxi-mum resolution 3,5 nm, enlargement from 18 to 300 000, tension increasing the electron flow 0,530 kV). Photos of the stone wool fibre and the product frag-
ments made during the research are presented in this paper.
2.2. Testing procedure
LST EN 826. Compression behaviour (compressive stress and/or compressive strength) of the mineral wool products are determined in accordance with the require-ments of the harmonised standards of the European Un-ion and Lithuania LST EN 826 . According to 6.1 of this standard, the test specimens of various dimensions of the mineral wool products may be chosen. The test specimens shall be squarely cut, the dimensions of the sides have to be from 50 mm 50 mm to 300 mm 300 mm. However, the test specimens width shall not be less than their thickness. According to the standard, the test specimens thickness must be the same as the original product thickness. Moreover, several test specimens shall not be put on each other in order not to modify the test specimen thickness .
Nevertheless, the standard for the factory made min-eral wool products EN 13162  indicates that the test specimens of the dimensions of only 200 mm 200 mm or 300 mm 300 mm may be chosen for testing. 5 meas-urements for one test result will be needed in the first case; whereas only 3 measurements in the second case. The surfaces of the specimens shall be prepared, ie sur-face grinded. The dimensions shall be determined with an accuracy of 0,5 %. The test shall be carried out at (23 5) C. Special conditioning of the test specimens is not necessary (however, the test specimens shall be stored at (23 5) C and relative humidity at (50 5) % at least 6 h prior to testing, if necessary).
In order to ensure a close contact between the plates of the equipment and the test specimen surface, the test specimen is preloaded with a pressure of (250 10) Pa.
A. Buska, R. Maiulaitis / JOURNAL OF CIVIL ENGINEERING AND MANAGEMENT 2007, Vol XIII, No 2, 97106 99
The test specimen compression period, ie force increasing rate, is dependent on the test specimen height, because it is compressed at a constant speed 0,1 d (d the thick-ness of test specimen expressed in mm) per min with a tolerance of 25 %.
The compression test is continued until the test specimen reaches the 10 % relative deformation. Thus, compressive stress (10) is determined at 10 % relative deformation. Compressive strength (m) is determined if the test specimen breaks up before reaching 10 % relative de